affecting the way cracks propagate. In front of a crack, a plastic zone can be present as the material yields. Beyond that region, the material remains elastic. The conditions for fracture are the most favorable at the boundary between this plastic and elastic zone, and thus cracks often initiate by the cleavage of a grain at that location. At low temperatures, where the material can become completely brittle, such as in a body-centered cubic (BCC) metal, the plastic zone shrinks away, and only the elastic zone exists. In this state, the crack will propagate by successive cleavage of the grains. At these low temperatures, the yield strength is high, but the fracture strain and crack tip radius of curvature are low, leading to a low toughness. At higher temperatures, the yield strength decreases, and leads to the formation of the plastic zone. Cleavage is likely to initiate at the elastic-plastic zone boundary, and then link back to the main crack tip. This is usually a mixture of cleavages of grains, and ductile fracture of grains known as fibrous linkages. The percentage of fibrous linkages increase as temperature increases until the linkup is entirely fibrous linkages. In this state, even though yield strength is lower, the presence of ductile fracture and a higher crack tip radius of curvature results in a higher toughness. Inclusions Inclusions in a material such as a second phase particles can act similar to brittle grains that can affect crack propagation. Fracture or decohesion at the inclusion can either be caused by the external applied stress or by the dislocations generated by the requirement of the inclusion to maintain contiguity with the matrix around it. Similar to grains, the fracture is most likely to occur at the plastic-elastic zone boundary. Then the crack can linkup back to the main crack. If the plastic zone is small or the density of the inclusions is small, the fracture is more likely to directly link up with the main crack tip. If the plastic zone is large, or the density of inclusions is high, additional inclusion fractures may occur within the plastic zone, and linkup occurs by progressing from the crack to the closest fracturing inclusion within the zone. Transformation toughening Transformation toughening is a phenomenon whereby a material undergoes one or more martensitic (displacive, diffusionless) phase transformations which result in an almost instantaneous change in volume of that material.